International Journal of Polymer Science
Volume 2018 (2018), Article ID 6387826, 10 pages
https://doi.org/10.1155/2018/6387826

Review Article

Analytical Methods to Characterize and Purify Polymeric Nanoparticles

Cristina Fornaguera¹ and Conxita Solans²

¹Grup d’Enginyeria de Materials, Institut Químic de Sarrià (IQS), Universitat Ramon Llull and Sagetis-Biotech, Via Augusta 390, 08017 Barcelona, Spain
²Institute of Advanced Chemistry of Catalonia (IQAC-CSIC) and Networking Centre on Bioengineering, Biomaterials and Nanomedicine (CIBER-BBN), C/Jordi Girona 18-26, 08034 Barcelona, Spain

Correspondence should be addressed to Cristina Fornaguera; cfornaguera@gmail.com

Received 30 June 2018; Accepted 10 July 2018; Published 5 August 2018

Academic Editor: Zhonghua Peng

Copyright © 2018 Cristina Fornaguera and Conxita Solans. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

Abstract.

Advances in polymeric nanoparticles as novel nanomedicines have opened a new class of diagnostic and therapeutic tools for many diseases. However, although the benchtop research studies in the nanoworld are numerous, their translation to currently marketed products is still limited. This lack of transference can be attributed, among other factors, to problems with nanomedicine characterization. Characterization techniques at the nanoscale could be divided in three categories: characterization of physicochemical properties (e.g., size and surface charge), characterization of nanomaterials interactions with biological components (e.g., proteins from the blood), and analytical characterization and purification methods. Currently available literature of this last group only describes methodologies applied for a specific type of nanomaterial or even methods used for bulk materials, which are not completely applicable to nanomaterials. For this reason, the current review aims to become a scholastic guide for those scientists starting in the nanoworld, giving them a description of analytical characterization techniques aimed to analyze polymers forming nanoparticles and possible forms to purify them before being used in preclinical and clinical applications.

1. Introduction

The field of nanotechnology and, more specifically, nanomedicine emerged about 20 years ago and since then, it experienced an exponential progress both in the fundamental study of nanosystems and in their multiple applications. Specifically, studies on polymeric nanoparticles have gained attention due to the multiple advantages that are attributed to this kind of nanosystems in terms of safety, versatility, and robustness [1–3]. Although the number of benchtop research studies developing novel nanosystems intended for biomedical applications is enormous, their use as clinically effective products is still limited. One of the main concerns of pharmaceutical industries for the production of novel formulations based on polymeric nanoparticles is the complexity of a deep characterization, which would enable their safe production and use in humans [4]. Therefore, a wide characterization of nanomedicines is a must before their testing in preclinical and clinical stages. However, the current technology is challenging in the sense that many characterization techniques have been applied directly from those methods used for bulk materials (not at the nanoscale) or using conditions that do not simulate biological environment [1, 2]. Therefore, many efforts must be devoted to the enhancement of the performance of current techniques. Nanomedicine characterization can be divided in three steps: first, an analytical characterization, useful for characterizing the materials they are composed of as well as to find out the impurities present and develop purification processes; second, a physicochemical characterization of the main parameters that will define the performance of nanomaterials in vivo, such as size, surface charge, and stability in biological conditions; and third, the study of their interaction with biological components (Figure 1). Although many reviews for the characterization of polymeric nanoparticles designed as nanomedicines exist, most of them give a particular point of view, signaling only some techniques [2, 5, 6]. Therefore, scientists working on the development of novel nanoformulations find themselves lost in the huge but dispersed existent bibliography. This is the reason that motivated the authors to write a series of three reviews with a scholastic character, to enable those scientists starting in the nanoworld to have guidelines for the correct characterization of polymeric nanoparticles. The first review was devoted to the characterization of nanomaterial interactions with biological systems [2]; the second one describes the physicochemical characterization techniques at the nanoscale, to assess size, surface charge, and stability of polymeric nanoparticles [7]; and the present one (third one) devoted to describe analytical characterization and purification techniques useful for nanomedicine study of polymeric nanoparticles (see a schematic representation of these techniques in the SI). Therefore, the purpose of the present review is to be a first practical guideline for those scientists initiating their studies in the nanoworld. It should be noted that it was not the objective of the authors to get deep into description of each individual technique but rather describe briefly each methodology to help the readers to select the most appropriate technique for their study and look for more specific information in the numerous references given for each technique.

Figure 1: Schematic representation of the process of nanomedicine characterization before translating to pharmaceutical production.

These methods have been classified not as a function of what is characterized but as a function of the technique: chromatographic, spectroscopic, calorimetric, and purification techniques. Authors will guide the reader through them with the objective to help in the selection of one or other technique depending on the parameter to study. Physicochemical techniques, mainly used to characterize size (e.g., light scattering or microscopy), are out of the scope of the present review [7].

2. Chromatographic Techniques

Chromatographic techniques, in general, are a group of techniques devoted to the separation of various compounds [8] as a step prior to their characterization. Their advantages are related with their high power of separation of substances, and the easy and simple manipulation, although they have as drawback the nonspecific interactions and the difficulty in method optimization [8, 9]. In this work, various types of chromatographic techniques are briefly described (Table 1). All of them could be also classified as purification techniques (see Section 5), since they are also able to separate compounds.

Table 1: Analytical chromatographic techniques.

Technique
Characteristics that analyses
Advantages
Disadvantages
References

Gel permeation chromatography (GPC)
Molecular weight
Rapid and simple
Interaction sample with column filling
Williams [10]

High resolution
Neverova and Van Eyk [8]

Cho et al. [1]

High-performance liquid chromatography (HPLC)
Quantification of actives
High resolution
Interaction sample with column filling
Neverova and Van Eyk [8]

Purification
Rapid and easy performance
Sapsford et al. [9]

Low cost/sample

Small sample volumes

Size exclusion chromatography (SEC)
Molecular weight
High resolution
Interaction sample with column filling
Kostanski et al. [25]

Rapid and simple
Need of a labelling tag
Sapsford et al. [9]

Rebolj et al. [26]

2.1. Gel Permeation Chromatography (GPC)

The gel permeation chromatography (GPC) is a widely used technique to determine the molecular weight of materials dissolved in organic solvents as well as the physical stability of assembled nanomaterials [1, 10]. The nanomaterials are eluted as a function of their molecular weight: the bigger the nanomaterials, the faster the elution. The quantification of the eluted samples is performed by means of UV-Vis absorption or changes in the refractive index.

This technique could be useful, for example, to study the stability of a polymer dissolved in an organic solvent. After various periods of time, the dissolved polymer should be analyzed through the GPC and its molecular weight assessed by using a calibration curve. Other examples of the use of GPC in the nanoscale could be the assessment of the polymer molecular weight, the degree of polymerization of a synthesized polymer, or even the number of monomer subunits that a polymer contains [11–14]. In some cases, GPC has also been used for the purification of quantum dots or carbon nanotubes, for example [15, 16].

GPC is advantageous in terms of short-time experiments. However, an important drawback of this technique is the possible interaction between the nanomaterials and the column filling, which could interfere the size assessment [1, 8].

2.2. High-Performance Liquid Chromatography (HPLC)

High-performance liquid chromatography (HPLC) is the most used type of chromatography not only for colloidal nanosystem studies but also for other type of materials (e.g., proteins). In the vast majority of studies, it is used for the fine quantification and separation (purification) of actives, such as drugs [5, 8, 9]. Briefly, it consists in the injection of the liquid sample using a pump that introduces it to a flow (mobile phase) that passes through a separative column (stationary phase), which entraps the molecules depending on their nature. The more interactions the molecules have with the column filling, the later they will be eluted. Further, molecules are eluted in a characteristic pattern for each compound. It results a chromatogram with the peaks of each compound (Figure 2).

Figure 2: Schematic representation of a HPLC system.

The quantification of the actives is required in any study of the encapsulation efficiency of drugs in the nanosystems or their release kinetics, as well as the percentage of conjugation to some nanosystems [9]. Examples of studies using HPLC for drug quantification exist are numerous [17–19]. For example, Fornaguera et al. [19] studied the encapsulation and release kinetics of dexamethasone (an anti-inflammatory drug) from polymeric nanoparticles. They were able to determine very low concentrations of the drug in a release study receptor solution, due to the high sensibility that offers the HPLC technique.

The resolution of the HPLC depends on the filling of the column (on the stationary phase properties), which is commonly composed of silica with attached alkyl chains, being the reversed phase C₁₈-type columns the most widely used, since it enables a differential retentionship depending on the polarity of the compounds [8, 9].

The advantages of HPLC are the high resolution, the low volumes required, and an easy, rapid, and economic manipulation [8, 9]. However, some drawbacks derived from the interaction of the samples with the stationary phase (column filing) could take place [9].

In 2004, it appeared the ultra-HPLC (UHPLC) technique, with many advantages among the traditional HPLC. It uses a column filling of particles of sub-2 micron size, while conventional HPLC uses particles between 2.5 and 5 microns. This reduction on the filling particle size enables a finer separation of similar compounds. In addition, the working pressure of UHPLC equipment is markedly higher than that supported by conventional HPLC, which enables more rapid flow rates, resulting in shorter elution times and decrease on the solvent amount used [20, 21].

2.3. Size Exclusion Chromatography (SEC)

Size exclusion chromatography (SEC), together with ion-exchange and affinity chromatography are classified as low-pressure liquid chromatography [9]. It is useful to characterize and separate (purify) nanomaterials with different properties, dispersed in an aqueous solution. For example, it has been useful to separate antibody-conjugated nanoparticles from the free antibody and nanoparticles [22, 23]. Another example of its use is the characterization of the molecular weight of nanoobjects, such as proteins or polymers [24]. The separation of the compounds depends not only on their molecular weight but also on their 3D dimensions, due to differences in pore permeation [25, 26]. It has the same advantages than other chromatographic techniques.

3. Spectroscopic Techniques

Spectroscopic techniques are those that give information on the interaction of an electromagnetic radiation with a sample, thus resulting in an absorption that depends on the excitation wavelength. Therefore, a wavelength spectrum with absorption/emission peaks that depend on the material is produced [9].

These techniques, summarized in Table 2, in general, are useful to characterize materials, which includes also nanomaterials, since spectra are characteristic of each material. A specific use of them, for example, could be the determination of the formation of bioconjugates between nanomaterials and conjugated moieties [9].

Table 2: Summary of the main advantages and disadvantages of spectroscopic techniques.

Technique
Use
Advantages
Disadvantages
References

Fourier transformed infrared (FTIR)
Chemical composition
Fast and inexpensive
Complicated sample preparation
Alben and Fiamingo [27]
Pretsch 2003
Sapsford et al. [9]
Lin et al. [5]

Characteristic of each material
Interference of water

Possible quantification
Relatively low sensitivity

Requires dried samples

Destructive

UV-Vis
Quantification of concentration
Cost effective
Interference between materials
Sapsford et al. [9]
Lin et al. 2014 [5]

Size and shape determination
Simple and fast

Useful for a variety of compounds

Fluorimetry
Quantitative fluorescence determination
High sensitivity Compound specificity
Limited to fluorescent compounds
Lakowicz [28]

Limited fluorescence lifetime

3.1. Infrared Spectroscopy

Fourier transformed infrared spectroscopy (FTIR) is a spectroscopic technique based on the measurement of vibrational transitions between different excitation states of molecules [27]. IR radiation is absorbed by molecules with dipoles that oscillate with the same frequency of the incident IR light. The IR absorption is an energy transfer of molecules and, if a change on their vibration occurs (by stretching, bending, or twisting of the bonds), the IR absorption changes; and this change can be characterized (e.g., covalent attachment of a carboxylic group to an amine group that results in an amide group) [5, 9].

It is a widely used technique, not only in the nanomedicine field but also in a variety of scientific fields. It has many advantages (Table 2), such as the fast and inexpensive performance and the obtaining of characteristic IR fingerprints of each compound, since they are a combination of the vibrational state of each atom [5]. In addition, it can be a quantitative tool in some specific conditions [27]. However, as drawbacks, there is the sample preparation (dried samples required, although some apparatus are prepared for liquid samples, but in this last case, a high concentration of the compounds to analyze is required), a requirement of technique optimization in most cases and interference with water molecules, which strongly absorb and need of a background signal [9]. Concerning nanomedicines experimentation, Sapsford et al. [9] and Lin et al., [5] for example, used FTIR to confirm the attachment of biomolecules onto nanomaterials surface, since FTIR results in a band pattern as a function of the chemical groups.

3.2. UV-Visible Spectroscopy

UV-Visible spectroscopy is a spectroscopy type that emits radiation of wavelength between 190 and 800 nm, widely used for the quantification of compounds concentration, and, in some cases, even size and shape, since each material absorbs at a determined wavelength and changes in the spectra could be related with changes in the aggregation of nanomaterials [5, 9]. It has been used, for example, to determine the conjugation and ratio of conjugation of biomolecules to nanomedicines [2, 5, 6, 8, 9].

It is a simple, fast, and cost-effective technique that can be applied to a variety of nanomaterials (Table 2). However, since most of the materials produce absorption at some wavelength, interferences between absorption of different compounds have to be taken into account [9].

3.3. Fluorimetry

Fluorimetry is a very sensitive spectroscopic technique that consists in the quantitative measurement of fluorescent signals, usually produced by aromatic molecules, for the detection and characterization of organic and inorganic compounds thanks to the application of a fluorescent laser to a sample (Figure 3) [28]. The fluorescent signal is composed of

(i)Excitation: it is produced by the absorption of the electromagnetic radiation by the sample to study.(ii)Losses of vibrational energy: they are produced after the absorption of energy and before the emission of fluorescence, due to the internal collision between the molecules of the sample.(iii)Emission: it consists of the energy produced by a molecule of the sample when it drops to a lower vibrational level (corresponding to lower energy and longer wavelengths), thus emitting energy in the form of fluorescence. The fluorescence is obtained as a spectrum and not a single band because not all the molecules of the sample drop to the same vibrational level.

Figure 3: Schematic representation of a fluorescence spectrophotometer model.

This technique has been used for various applications, all of them taking advantage of the capacity of the studied materials to be excited under a fluorescent laser and emit fluorescence of another wavelength. For example, Lin et al. [5] used fluorescence to study conformational changes of biomaterials and their conjugation with nanomaterials. Fornaguera et al. [29], in contrast, took advantage of the fluorescent properties of galantamine drug to quantify its encapsulation efficiency in polymeric nanoparticles and its release. Chen et al. [30] used fluorimetry to confirm covalent bond formation onto polymeric nanoparticle surface. In addition, since the excitation/emission are wavelength specific, it can be also used to quantify two colocalized fluorescent dyes, due to the simultaneous detection of the different wavelengths.

Although the varied uses of fluorescence, it has two main drawbacks (Table 2): only some materials have fluorescence and the fluorescence lifetime is limited, with a wavelength dependent on the specific compound [28].

Recently, advanced techniques combining the advantages of fluorescent signal have appeared. Of special importance is the Förster resonance energy transfer or FRET technology. It consists in the combination of two fluorescent probes labeling pairs of two compounds, the first one called the donor and the second one called the acceptor. Fluorescence of excitation wavelength of the donor is directed to the compound, which, under the specific fluorescence will emit fluorescence in another wavelength. The acceptor is excited specifically by the emission wavelength of the donor (energy transference) and emits fluorescence in another wavelength. Therefore, if both compounds are very close (<10 nm), when exciting the donor, only fluorescence signal of the acceptor emission wavelength will be detected. In contrast, if both molecules are not close enough, when exciting the donor, fluorescence emission of this donor wavelength will be detected. Therefore, this technique is very useful to study two compound aggregation, and it is starting to play an important role in nanosystem studies [31–33]. Lai et al. [31], for example, studied the drug release from porous silica nanoparticles using this technique. Liu et al. [32], in contrast, used FRET technology as a nanodiagnostic system to detect the presence of chrome in urine, which produces the dissociation of FRET pairs, specifically designed for this purpose.

4. Calorimetric Techniques

Calorimetric techniques are a type of techniques that apply a temperature change to the samples to study physical phenomena, such as the crystalline transition, fusion, vaporization, sublimation, absorption, adsorption, and desorption and chemical phenomena, such as chemisorptions, desolvation, decomposition, oxidative degradation, solid-state, and solid-gas reactions [34]. Two main calorimetric techniques will be described in this review (Table 3).

Table 3: Summary of the main advantages and disadvantages of calorimetric techniques.

Technique
Use
Advantages
Disadvantages
References

Differential scanning calorimetry (DSC)
Glass transition
Melting temperature
Low amounts of sample
High precision and sensitivity
Requires sample preparation
Requires an appropriate reference
Hunt [36]
Haq [35]
Lu and Li [37]
Sapsford et al. [9]

Thermogravimetry (TGA)
Weight loss
Low amounts of sample
High precision and sensitivity
Requires sample preparation
Requires an appropriate reference
Berger et al. [38]
Sapsford et al. [9]
Lin et al. [5]

4.1. Differential Scanning Calorimetry (DSC)

Differential scanning calorimetry (DSC) is a technique that continuously measures the apparent specific heat of a system as a function of the temperature [35]. It is useful for the measurement of the glass transition and melting temperatures of materials including nanosystems. The glass transition temperature (Tg) is the temperature at which a material in a solid state changes its conformation. The melting temperature is always higher than the Tg [36, 37]. Therefore, in some cases, the determination of the melting temperature is not performed because it requires too high temperatures.

It is a useful technique to determine the structure and stability of nanomaterials, as well as their conformation, since material transitions will change depending on the nanomaterial composition [5, 35].

4.2. Thermogravimetric Assays (TGA)

Thermogravimetric assays (TGA) are another type of calorimetric techniques which measure the weight loss of the samples [34, 38].

It is a useful technique to determine the amount of nanoconjugation, since the change on the nanomaterial composition produces changes in the temperature weight loss [5, 9]. For example, Fornaguera et al. [39] used TGA analysis to confirm the covalent attachment of a dendritic carbosilane wedge to polymeric nanoparticles.

Since both calorimetric techniques have a similar performance, their advantages and disadvantages have been summarized together. Calorimetric techniques are advantageous in terms of small amount of sample required, high precision and sensitivity. However, an appropriate reference as well as the preparation of the sample is required [9, 35, 38].

5. Purification Techniques

The composition of colloidal nanomaterials is a key point, since it affects not only its transport, delivery, and biodistribution in vivo, but, most importantly, it can contribute to toxicity-related problems [4–6, 9]. For this reason, to ensure a safe formulation, free of contaminants, a purification step is strongly recommended, followed by a physicochemical characterization, before starting preclinical and clinical analysis.

Although various methods exist for the colloidal nanomaterial purification, such as the magnetic separation for magnetic nanoparticles, for example [40, 41], in most cases, when nanosystems do not possess any specific inherent property that facilitates purification, this step may represent a difficult and tedious process, being sometimes impossible to confirm the presence of a purified compound [9]. In the following, common purification techniques, useful for a variety of nanosystems, are summarized (Table 4). Specific techniques, useful only for a determined material have not been described in this review.

Table 4: Summary of the main advantages and disadvantages of the described purification techniques.

Technique
Use
Advantages
Disadvantages
References

Filtration
Purification
Useful for thermolabile compounds
Time consuming
Scopes [44]

Sterilization

Concentration
Rapid and simple
Bigger sizes determined by the cut-off size
Sapsford et al. [9]

Dispersant changement
Commercially available devices
Single-use devices
Roy et al. [43]

Reduce size polydispersity
Cost effective
Dobrovolskaia and McNeil [42]

Centrifugation
Purification
High efficiency
Special equipment required for large volumes
Scopes [44]

Concentration
Rapid, facile, and economic
Difficult to resuspend soft matter
Sapsford et al. [9]

Dispersant changement
Low amounts of sample

Appropriate for different kinds of nanomaterials

Dialysis
Purification
Rapid, facile, and economic
Limited to the membranes MWCO
Vauthier et al. [46]

Concentration
Commercially available devices
High receptor solution volumes
Sapsford et al. [9]

Dispersant changement
No sample pretreatment

Electrophoresis
Purification
Simple and economic
Postelectrophoresis purification steps
Sapsford et al. [9]

Jason [51]

High resolution and sensitivity

Need of charged compounds
Scopes [45]

It is worth remarking the contamination by endotoxins. Although methodology to purify from endotoxins is out of the scope of the present review, authors would like to remark the importance of producing nanomedicines clean from this type of contamination, which could be produced from many lipopolysaccharides, of the omnipresent Gram-negative bacteria. It is important to clean all material used before starting the production (e.g., by cleaning with sodium hydroxide or heating treatments) of nanomedicines and to confirm that resulting nanomedicines are clean from endotoxins [6].

5.1. Filtration

Filtration is a purification method, specifically used to sterilize nanomaterial colloidal dispersions. This method is advantageous as a sterilization technique for thermolabile compounds [42]. In addition, it represents a rapid, commercially available, cost-effective, and simple technique. Although it can be performed under atmospheric pressure, usually, it is performed taking advantage of special devices with filters, which are centrifuged, thus increasing the speed and efficiency of the process [9, 43]. An aspect that could be considered as a drawback is that filtration of large volumes could produce clogging of the filters, reason for which filters are single-use devices [44].

In addition, it can also be useful for other purposes, such as for the concentration of colloid nanomedicines or the reduction of their polydispersity. For example, Roy et al. [43] produced Au and CdS nanoparticles and passed them through a multiwall carbon nanotube, which was used as a filter to control the maximum nanoparticle size, thus eliminating the bigger ones and reducing nanoparticle size polydispersity [43, 45–50].

5.2. Centrifugation

Centrifugation is another technique useful for the purification of nanomaterials. It consists of the application of a centrifugal force to enhance the precipitation of nanomaterials due to the increased gravitational field [44]. Different kinds of centrifugation exist, such as the conventional centrifugation, ultracentrifugation, and gradient centrifugation, whose use depends on the objective of the study and on the nanomaterials type, specifically on their size [9].

Centrifugation is more efficient than filtration. It is a rapid, facile, and economic technique, able to be used for different kinds of nanomedicines. In addition, low amounts of sample are required. However, the centrifugation of large volumes requires special equipment and in some cases, difficulties on resuspending sediment nanomaterials appear, specifically when working with soft matter, which are not always possible to recover their dispersion liquid state [9, 44].

Apart from the use of centrifugation to purify nanomedicines, it has been also used to concentrate nanomedicines, to change their dispersant, and to separate conjugated nanomaterials from those nonconjugated [9]. For example, Fornaguera et al. [19] centrifuged PLGA nanoparticles to purify them from the surfactant traces and to concentrate them.

5.3. Dialysis

Dialysis consist on changing the nanomaterial dispersant by means of submerging a semipermeable dialysis bag (or a dialysis dispositive) filled with the nanomaterial dispersion, in a receptor solution. Therefore, it is not only useful for the nanomaterial purification but also for nanomedicine concentration and to change the dispersant to achieve the desired properties (e.g., dialysis with PBS to achieve the physiological pH and osmolality). The liquid diffuses through the membrane from the more concentrated solution (sample or receptor solution) to the less concentrated one, to achieve an osmotic equilibrium. Therefore, osmotic conditions have to be completely controlled to avoid volume changes; except in the case of nanosystem concentration, where a decrease of the sample volume is required and it can be achieved using a hypotonic receptor solution [9]. It is worth noting that not only the liquid but also molecules with smaller molecular weight than the molecular weight cut-off of the membrane can also diffuse to achieve the osmotic equilibrium. For example, Vauthier et al. [46] used and demonstrated inverse dialysis as an appropriate methodology to concentrate polymeric nanoparticles using a receptor solution with a high osmotic pressure.

This technique is advantageous in terms of minimal sample manipulation, without the need of any pretreatment, but it is limited to the existent dialysis membranes. If the sample to dialyse is expected to interact with the membrane or if the molecular weight cut-off is not appropriate, this technique cannot be used. In addition, high volumes of the receptor solution are usually required [9, 46].

5.4. Electrophoresis

Electrophoretic techniques consist of the application of an electric field to a polymeric gel (composed mainly of agarose or polyacrylamide) submerged in a liquid buffer; through which charged molecules run depending on their charge and/or on their molecular weight. Although electrophoresis is used with many objective, one of the uses of this technique is the separation and purification of determined nanomaterials, which has been widely reported [9]. General examples of the purification use of electrophoresis are the following. Meyer et al. [47] reported the use of PAGE (polyacrylamide gel) electrophoresis for the purification of RNAs extracted from enzymatic synthesis or from cells, for example. They also demonstrated both native and denaturing electrophoretic conditions for the selection of RNAs of the required size.

The main advantages of this technique are its economic and simple performance together with the high resolution and sensitivity. However, only charged compounds can be purified through electrophoresis, and once the compound is separated in the gel, further purification steps are required to extract it from the gel [9, 45, 51].

Although it is not specifically a technique for the purification of nanosystems, it was considered appropriate to remark an electrophoretic type widely used to characterize the formation of nanocomplexes by the electrostatic interactions between their components. This technique is called electrophoretic mobility shift assay (EMSA). EMSA consists in a native (nondenaturing) polyacrylamide electrophoresis where samples migrate depending on their charge, under an electric field [48]. It is widely used in the nanomedicine field for the determination of the complexation ratio between two compounds, for example, polymeric nanoparticles and antisense oligonucleotides (Figure 4) [39]. The complexation is detected due to a retardation of the oligonucleotide band migration when complexes are formed, since complexes migrate slower than free nucleic acids [48].

Figure 4: Example of an EMSA of polymeric nanoparticles conjugated with antisense oligonucleotides at different nanoparticle/oligonucleotide (N/P) charge ratios. When the complexation is achieved (zero surface charge), the band is diffused (at 0.75/1 in this case).

Its rapid performance, simplicity, robustness, and high sensitivity make this methodology the choice for the study of electrostatic complexes formation of a wide range of compounds. Although EMSA is usually applied as a qualitative technique, under the appropriate conditions, it can be also useful to quantify the stoichiometry of complexation. It is also remarkable that multiple EMSA variants exist for various purposes, such as the time-course EMSA to measure the dissociation kinetics or the circular permutation to measure the DNA bending [48–50]. However, EMSA has also some disadvantages, such as the performance of the assay in nonchemical equilibrium [48].

6. Conclusions

A complete characterization of nanomaterials intended for biomedical purposes (diagnostic, treatment, or theragnostic) is a must before the translation to preclinical and clinical studies. Classical chemistry analytical techniques can be applied for the characterization of some aspects of nanomaterials, since nanomaterial properties usually change from those of their components. Chromatographic techniques can be useful for the determination of the molecular weight of nanosystems, as well as for the purification of the produced nanoobject from raw materials and impurities. Spectroscopic techniques, in parallel, can be very useful for the confirmation of the formation of the nanosystems, assessing the materials of which it is composed as well as its aggregation/attachment state. Calorimetric techniques can be useful for the study of the nanomaterial behavior when submitting them to temperature changes. Finally, it is always required a purification step to ensure the obtaining of a safe nanosystem, free of impurities and raw materials. Therefore, as a general conclusion of this review, it is strongly recommended to take a look on the variety of existent techniques to look for all the aspects that must be known before the translation of a novel nanomaterial to a human diagnostic or therapeutic formulation.

Conflicts of Interest

The authors declare that they have no conflicts of interest.

Acknowledgments

This work was funded by Spanish Ministry of Economy and Competitivity, MINECO (grant CTQ2014-52687) and Generalitat de Catalunya (grant 2014-SGR-1655). CIBER-BBN is an initiative funded by the VI National R&D&I Plan 2008–2011, Iniciativa Ingenio 2010, Consolider Program, CIBER Actions and financed by the Instituto de Salud Carlos III with assistance from the European Regional Development Fund. Cristina Fornaguera is grateful to MINECO for their PTQ2015 grant.

Supplementary Materials

Schematic representation of analytical techniques to characterize a nanoparticle dispersion, as a summary of the whole review. (Supplementary Materials)

References

E. J. Cho, H. Holback, K. C. Liu, S. A. Abouelmagd, J. Park, and Y. Yeo, “Nanoparticle characterization: state of the art, challenges, and emerging technologies,” Molecular Pharmaceutics, vol. 10, no. 6, pp. 2093–2110, 2013.

C. Fornaguera and C. Solans, “Methods for the in vitro characterization of nanomedicines—biological component interaction,” Journal of Personalized Medicine, vol. 7, no. 1, p. 2, 2017.

N. Segovia, P. Dosta, A. Cascante, V. Ramos, and S. Borrós, “Oligopeptide-terminated poly (β-amino ester) s for highly efficient gene delivery and intracellular localization,” Acta Biomaterialia, vol. 10, no. 5, pp. 2147–2158, 2014.

M. A. Dobrovolskaia, M. Shurin, and A. A. Shvedova, “Current understanding of interactions between nanoparticles and the immune system,” Toxicology and Applied Pharmacology, vol. 299, pp. 78–89, 2016.

P. C. Lin, S. Lin, P. C. Wang, and R. Sridhar, “Techniques for physicochemical characterization of nanomaterials,” Biotechnology Advances, vol. 32, no. 4, pp. 711–726, 2014.

R. M. Crist, J. H. Grossman, A. K. Patri et al., “Common pitfalls in nanotechnology: lessons learned from NCI’s Nanotechnology Characterization Laboratory,” Integrative Biology, vol. 5, no. 1, pp. 66–73, 2012.

C. Fornaguera and C. Solans, “Characterization of polymeric nanoparticle dispersions for biomedical applications: size, surface charge and stability,” Pharmaceutical Nanotechnology, vol. 6, 2018.

I. Neverova and J. E. Van Eyk, “Role of chromatographic techniques in proteomic analysis,” Journal of Chromatography, B: Analytical Technologies in the Biomedical and Life Sciences, vol. 815, no. 1-2, pp. 51–63, 2005.

K. E. Sapsford, K. M. Tyner, B. J. Dair, J. R. Deschamps, and I. L. Medintz, “Analyzing nanomaterial bioconjugates: a review of current and emerging purification and characterization techniques,” Analytical Chemistry, vol. 83, no. 12, pp. 4453–4488, 2011.

T. Williams, “Gel permeation chromatography: a review,” Journal of Materials Science. Materials in Medicine, vol. 5, no. 9, pp. 811–820, 1970.

H. Determann, Chromatography Gel Filtration, Gel Permea, Springer Science and Business Media, 2012.

J. C. Moore, “Gel permeation chromatography. I. A new method for molecular weight distribution of high polymers,” Journal of Polymer Sciences, vol. 2, pp. 835–843, 1964.

E. Temyanko, P. S. Russo, and H. Ricks, “Study of rodlike homopolypeptides by gel permeation chromatography with light scattering detection: validity of universal calibration and stiffness assessment,” Macromolecules, vol. 34, no. 3, pp. 582–586, 2001.

A. Rahimi, A. Ulbrich, J. J. Coon, and S. S. Stahl, “Formic-acid-induced depolymerization of oxidized lignin to aromatics,” Nature, vol. 515, no. 7526, pp. 249–252, 2014.

Y. Shen, M. Y. Gee, R. Tan, P. J. Pellechia, and A. B. Greytak, “Purification of quantum dots by gel permeation chromatography and the effect of excess ligands on shell growth and ligand exchange,” Chemistry of Materials, vol. 25, no. 14, pp. 2838–2848, 2013.

B. S. Flavel, K. E. Moore, M. Pfohl, M. M. Kappes, and F. Hennrich, “Separation of single-walled carbon nanotubes with a gel permeation chromatography system,” ACS Nano, vol. 8, no. 2, pp. 1817–1826, 2014.

T. Radhakrishna, D. S. Rao, and G. O. Reddy, “Determination of pioglitazone hydrochloride in bulk and pharmaceutical formulations by HPLC and MEKC methods,” Journal of Pharmaceutical and Biomedical Analysis, vol. 29, no. 4, pp. 593–607, 2002.

A. E. Gulyaev, S. E. Gelperina, I. N. Skidan, A. S. Antropov, G. Y. Kivman, and J. Kreuter, “Significant transport of doxorubicin into the brain with polysorbate 80-coated nanoparticles,” Pharmaceutical Research, vol. 16, no. 10, pp. 1564–1569, 1999.

C. Fornaguera, M. Llinàs, C. Solans, and G. Calderó, “Design and in vitro evaluation of biocompatible dexamethasone-loaded nanoparticle dispersions, obtained from nano-emulsions, for inhalatory therapy,” Colloids and Surfaces B: Biointerfaces, vol. 125, pp. 58–64, 2015.

J. Cielecka-Piontek, P. Zalewski, A. Jelińska, and P. Garbacki, “UHPLC: the greening face of liquid chromatography,” Chromatographia, vol. 76, no. 21-22, pp. 1429–1437, 2013.

S. Fekete, J. Schappler, J.-L. Veuthey, and D. Guillarme, “Current and future trends in UHPLC,” TrAC Trends in Analytical Chemistry, vol. 63, pp. 2–13, 2014.

K. Ulbrich, T. Hekmatara, E. Herbert, and J. Kreuter, “Transferrin- and transferrin-receptor-antibody-modified nanoparticles enable drug delivery across the blood-brain barrier (BBB),” European Journal of Pharmaceutics and Biopharmaceutics, vol. 71, no. 2, pp. 251–256, 2009.

S. Wagner, F. Rothweiler, M. G. Anhorn et al., “Enhanced drug targeting by attachment of an anti αv integrin antibody to doxorubicin loaded human serum albumin nanoparticles,” Biomaterials, vol. 31, no. 8, pp. 2388–2398, 2010.

M. Sadao and H. G. Barth, Size Exclusion Chromatography, Springer Science and Business Media, 2013.

L. K. Kostanski, D. M. Keller, and A. E. Hamielec, “Size-exclusion chromatography - a review of calibration methodologies,” Journal of Biochemical and Biophysical Methods, vol. 58, no. 2, pp. 159–186, 2004.

K. Rebolj, D. Pahovnik, and E. Žagar, “Characterization of a protein conjugate using an asymmetrical-flow field-flow fractionation and a size-exclusion chromatography with multi-detection system,” Analytical Chemistry, vol. 84, no. 17, pp. 7374–7383, 2012.

J. Alben and F. Fiamingo, “Fourier transformed infrared spectroscopy,” in Optical Techniques in Biological Research, D. Rousseau, Ed., pp. 133–178, Bell telephone laboratories Inc., 1984.

J. Lakowicz, Principles of Fluorescence Spectroscopy, Springer, 2010.

C. Fornaguera, N. Feiner-Gracia, G. Calderó, M. J. Garcia-Celma, and C. Solans, “Galantamine-loaded PLGA nanoparticles, from nano-emulsion templating, as novel advanced drug delivery systems to treat neurodegenerative diseases,” Nanoscale, vol. 7, no. 28, pp. 12076–12084, 2015.

H. Chen, J. Gao, Y. Lu et al., “Preparation and characterization of PE38KDEL-loaded anti-HER2 nanoparticles for targeted cancer therapy,” Journal of Controlled Release, vol. 128, no. 3, pp. 209–216, 2008.

J. Lai, B. P. Shah, E. Garfunkel, and K. Lee, “Energy transfer-based mesoporous silica nanoparticles for real-time monitoring of drug release,” ACS Nano, vol. 7, no. 3, pp. 2741–2750, 2013.

B. Liu, H. Tan, and Y. Chen, “Upconversion nanoparticle-based fluorescence resonance energy transfer assay for Cr (III) ions in urine,” Analytica Chimica Acta, vol. 761, pp. 178–185, 2013.

J. Shi, F. Tian, J. Lyu, and M. Yang, “Nanoparticle based fluorescence resonance energy transfer (FRET) for biosensing applications,” Journal of Materials Chemistry B, vol. 3, no. 35, pp. 6989–7005, 2015.

A. Coats and J. Redfern, “Thermogravimetric analysis,” The Analyst, vol. 88, no. 1053, pp. 906–924, 1963.

I. Haq, D. Chowdhry, and T. Jenkins, “Calorimetric techniques in the study of high-order DNA-drug interactions,” Methods in Enzymology, vol. 340, pp. 109–149, 2001.

A. Hunt, “A simple connection between the melting temperature and the glass temperature in a kinetic theory of the glass transition,” Journal of Physics. Condensed Matter, vol. 4, no. 32, pp. L429–L431, 1992.

Z. Lu and J. Li, “Correlation between average melting temperature and glass transition temperature in metallic glasses,” Applied Physics Letters, vol. 94, no. 6, article 061913, 2009.

R. Berger, H. P. Lang, C. Gerber et al., “Micromechanical thermogravimetry,” Chemical Physics Letters, vol. 294, no. 4-5, pp. 363–369, 1998.

C. Fornaguera, S. Grijalvo, M. Galán et al., “Novel non-viral gene delivery systems composed of carbosilane dendron functionalized nanoparticles prepared from nano-emulsions as non-viral carriers for antisense oligonucleotides,” International Journal of Pharmaceutics, vol. 478, no. 1, pp. 113–123, 2015.

M. Colombo, S. Carregal-Romero, M. F. Casula et al., “Biological applications of magnetic nanoparticles,” Chemical Society Reviews, vol. 41, no. 11, pp. 4306–4334, 2012.

L. H. Reddy, J. L. Arias, J. Nicolas, and P. Couvreur, “Magnetic nanoparticles: design and characterization, toxicity and biocompatibility, pharmaceutical and biomedical applications,” Chemical Reviews, vol. 112, no. 11, pp. 5818–5878, 2012.

M. A. Dobrovolskaia and S. E. McNeil, “Handbook of immunological properties of engineered nanomaterials,” in Frontiers in Nanobiomedical Research, SAIC-Frederick Inc., 1st edition, 2013.

S. Roy, V. Jain, R. Bajpai et al., “Formation of carbon nanotube bucky paper and feasibility study for filtration at the nano and molecular scale,” Journal of Physical Chemistry C, vol. 116, no. 35, pp. 19025–19031, 2012.

R. Scopes, Protein Purification: Principles and Practice, Springer, New York, NY, USA, 1994.

R. K. Scopes, Protein Purification: Principles and Practice, Springer Science and Business Media, 2013.

C. Vauthier, B. Cabane, and D. Labarre, “How to concentrate nanoparticles and avoid aggregation?” European Journal of Pharmaceutics and Biopharmaceutics, vol. 69, no. 2, pp. 466–475, 2008.

M. Meyer and B. Masquida, “Polyacrylamide gel electrophoresis for purification of large amounts of RNA,” in Nucleic Acid Crystallography, E. Ennifar, Ed., vol. 1320 of Methods in Molecular Biology, Humana Press, New York, NY, USA, 2016.

L. M. Hellman and M. G. Fried, “Electrophoretic mobility shift assay (EMSA) for detecting protein-nucleic acid interactions,” Nature Protocols, vol. 2, no. 8, pp. 1849–1861, 2007.

J. Gerstle and M. G. Fried, “Measurement of binding kinetics using the gel electrophoresis mobility shift assay,” Electrophoresis, vol. 14, no. 1, pp. 725–731, 1993.

D. Senear and M. Brenowitz, “DNA bending in protein-DNA complexes,” Methods in Enzymology, vol. 208, pp. 118–146, 1991.

J. C. Jason, Protein Purification: Principles, High Resolution Methods, and Applications, John Wiley and Sons, 2012.